bio-inspired self-healing structural color hydrogel bio-inspired self-healing structural color...
Post on 06-Jun-2020
Embed Size (px)
Bio-inspired self-healing structural color hydrogel Fanfan Fua,1, Zhuoyue Chena,1, Ze Zhaoa, Huan Wanga, Luoran Shanga, Zhongze Gua, and Yuanjin Zhaoa,2
aState Key Laboratory of Bioelectronics, School of Biological Science and Medical Engineering, Southeast University, Nanjing 210096, China
Edited by David A. Weitz, Harvard University, Cambridge, MA, and approved April 24, 2017 (received for review March 3, 2017)
Biologically inspired self-healing structural color hydrogels were developed by adding a glucose oxidase (GOX)- and catalase (CAT)-filled glutaraldehyde cross-linked BSA hydrogel into metha- crylated gelatin (GelMA) inverse opal scaffolds. The composite hydrogel materials with the polymerized GelMA scaffold could maintain the stability of an inverse opal structure and its resultant structural colors, whereas the protein hydrogel filler could impart self-healing capability through the reversible covalent attachment of glutaraldehyde to lysine residues of BSA and enzyme additives. A series of unprecedented structural color materials could be cre- ated by assembling and healing the elements of the composite hydrogel. In addition, as both the GelMA and the protein hydro- gels were derived from organisms, the composite materials pre- sented high biocompatibility and plasticity. These features of self- healing structural color hydrogels make them excellent functional materials for different applications.
colloidal crystal | self-healing | inverse opal | structural color | hydrogel
Structural colors, arising from intrinsic periodic nanostructuresand resulting in the interaction of light with these photonic nanostructures, have attracted much interest because of the fasci- nation associated with the display of various brilliant examples (1– 6). The creatures displaying brilliant structural colors are prevalent in nature, and their life, including communication, shielding, and other biological functions, is closely linked with these structural colors (7). Researchers, marveling at these miracles, have devoted their work to bio-inspired structure colors materials. Structural color hydrogels are one of the most important examples and have been widely studied and used in switches (8, 9), optical devices (10, 11), sensing materials (12, 13), and wearable electronics (14), etc. (15– 20). However, because the deterioration and accumulation of damage of these materials during applications are inevitable, to achieve next-generation materials for both fundamental research and practical applications, the creation of bio-inspired structural color materials with increased survivability is still necessary. Coincidentally, for the purpose of increasing the survivability
and lifetime of an organism, the function of self-healing that can spontaneously heal injury and recover functionality in creatures is ubiquitous in nature (21–25). Inspired by these creatures, re- searchers have developed numerous self-healing hydrogel mate- rials that fuse together with their homogeneous hydrogels for various important applications (26–37). However, the fusion pro- cess of the self-healing hydrogels could also happen in their neighboring nanostructures; this would cause the destruction of the periodic photonic scaffolds. Therefore, a self-healing hydrogel with stable structural color has not yet been reported, and its construction remains a challenge. In this paper, we present the desired self-healing structural color
hydrogels by constructing them with a composite nanostructure, as indicated in Fig. 1. This nanostructure was composed of a meth- acrylated gelatin (GelMA) hydrogel inverse opal scaffold and a filler of glutaraldehyde cross-linked BSA hydrogel with enzyme additives of glucose oxidase (GOX) and catalase (CAT). The polymerized GelMA hydrogel scaffold in the composite materials could guaran- tee the stability of both the inverse opal structure and its resultant structural colors, whereas the protein hydrogel filler could impart the materials with self-healing capability through the reversible covalent attachment of the glutaraldehyde to lysine residues of BSA and the
enzyme additives. As both the GelMA and protein hydrogels are derived from organisms, the composite materials had high bio- compatibility and plasticity. It was demonstrated that a series of new structural color materials with one-dimensional (1D) linear microfiber, 2D pattern, and 3D photonic path structures could be developed by assembling and healing the composite structural color hydrogel elements. These features make our self-healing structural color hydrogels highly promising for different applica- tions, such as counterfeit prevention, integrated optics, and biomedical engineering.
Results and Discussion In a typical experiment, the GelMA hydrogel inverse opal scaf- folds were fabricated by replicating silica colloidal crystal tem- plates. These colloidal crystal templates were prepared by the self-assembly of silica nanoparticles in silica capillaries or on glass slides, which closely packed and finally formed an ordered structure during dehydration (Fig. 2A). This ordered packing of the nanoparticles endowed the colloidal crystals with inter- connected nanopores throughout the templates, which enabled infiltration of the GelMA pregel solution. After the pregel so- lution penetrated the nanopores and filled all of the voids of the templates by capillary action, the solution was polymerized to form a hydrogel by UV light. Finally, the inverse opal scaffolds were obtained by etching the silica nanoparticles, leaving an in- verse opal GelMA hydrogel scaffold (Fig. 2B). This kind of scaffold displays various brilliant structure colors (Fig. S1), which is an important feature of the materials. To impart to the structural color hydrogel the capability of
self-healing, the glutaraldehyde cross-linked BSA hydrogel with enzyme additives of GOX and CAT was filled into the inverse opal scaffold. In this process, the pregel was first prepared with a
Structural color hydrogels have been widely studied and used in different applications, such as in switches, optical devices, etc. However, because the deterioration and accumulation of damage of these materials are inevitable during applications, the creation of bio-inspired structure color materials with in- creased survivability is still desired for both fundamental re- search and practical applications. In this study, inspired by creatures in nature with spontaneous healing from injury and recovering of functionality, we demonstrated a self-healing structural color hydrogel by filling a healable protein hydro- gel into an inverse opal scaffold. A series of new structural color materials with 1D linear microfiber, 2D pattern, and 3D photonic path structures could be constructed by assembling and healing the composite structural color hydrogel elements.
Author contributions: Y.Z. designed research; F.F. and Z.C. performed research; F.F., Z.C., Z.Z., H.W., L.S., Z.G., and Y.Z. analyzed data; F.F. and Y.Z. wrote the paper; Z.Z. contrib- uted to scientific discussion; and H.W. and L.S. contributed to scientific discussion of the article.
The authors declare no conflict of interest.
This article is a PNAS Direct Submission. 1F.F. and Z.C. contributed equally to this work. 2To whom correspondence should be addressed. Email: email@example.com.
This article contains supporting information online at www.pnas.org/lookup/suppl/doi:10. 1073/pnas.1703616114/-/DCSupplemental.
5900–5905 | PNAS | June 6, 2017 | vol. 114 | no. 23 www.pnas.org/cgi/doi/10.1073/pnas.1703616114
http://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1703616114/-/DCSupplemental/pnas.201703616SI.pdf?targetid=nameddest=SF1 http://crossmark.crossref.org/dialog/?doi=10.1073/pnas.1703616114&domain=pdf mailto:firstname.lastname@example.org http://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1703616114/-/DCSupplemental http://www.pnas.org/lookup/suppl/doi:10.1073/pnas.1703616114/-/DCSupplemental www.pnas.org/cgi/doi/10.1073/pnas.1703616114
protein concentration of 13.5 wt% (GOX, CAT, and BSA for 0.2%, 0.8%, and 12.5%, respectively). The concentration of glutaraldehyde was 0.5 wt%, and the pH of the solution was adjusted to 7.0. To fully fill the protein hydrogel into the nano- pores of the inverse opal, the structure color hydrogels should be dehydrated and then immersed in the pregel solution in a vac- uum environment. After these steps, the structure color hydro- gels were transferred to a closed environment with a certain humidity for the polymerization of the infiltrated pregel in the inverse opals (Fig. 2C). Finally, a hybrid inverse opal hydrogel with brilliant structure color was achieved. The formation of the structural colors of the hydrogels was
ascribed to their orderly arranged nanostructure, which imparts to the inverse opal hydrogel and its derived hybrid hydrogel a unique photonic band gap (PBG). This PBG leads light with certain wavelengths or frequencies to be located in and reflected instead of propagating through the materials. As a result, the colloidal crystal templates and the inverse opal scaffold, together with the hybrid hydrogel, all showed vivid colors and possessed character- istic reflection peaks. Under normal incidence, the main reflection peak position λ of these materials can be estimated by Bragg’s equation, λ = 2d111naverage, where d111 is the interplanar distance of the (111) diffracting planes, and naverage refers to the average refractive index of the materials. Although the infiltration of the protein hydrogel into the inverse opal could increase the naverage of the hybrid material, the d111-related